#------------------------------------------------------------------------------
#$Date: 2015-05-30 05:06:12 +0300 (Sat, 30 May 2015) $
#$Revision: 137550 $
#$URL: svn://www.crystallography.net/cod/cif/2/01/99/2019970.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2019970
loop_
_publ_author_name
'Stetskiv, Andrij'
'Rozdzynska-Kielbik, Beata'
'Misztal, Renata'
'Pavlyuk, Volodymyr'
_publ_section_title
;
 Grown from lithium flux, the ErCo₅Si~3.17~ silicide is a combination of
 disordered derivatives of the UCo₅Si₃ and Yb₆Co₃₀P₁₉ structure
 types
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              506
_journal_page_last               510
_journal_paper_doi               10.1107/S2053229615009791
_journal_volume                  71
_journal_year                    2015
_chemical_formula_iupac          'Er Co5 Si3.17'
_chemical_formula_moiety         '6(Co5 Er Si3), 2(Si0.50)'
_chemical_formula_sum            'Co30 Er6 Si19'
_chemical_formula_weight         3305.17
_chemical_name_systematic
;
Hexaerbium triacontacobalt enneakaidecasilicide
;
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   14.88410(10)
_cell_length_b                   14.88410(10)
_cell_length_c                   3.68500(10)
_cell_measurement_reflns_used    10399
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      28.27
_cell_measurement_theta_min      4.18
_cell_volume                     706.99(2)
_computing_cell_refinement
;
CrysAlis CCD (Oxford Diffraction, 2008)
;
_computing_data_collection
;
CrysAlis CCD (Oxford Diffraction, 2008)
;
_computing_data_reduction
;
CrysAlis RED (Oxford Diffraction, 2008)
;
_computing_molecular_graphics
;
DIAMOND (Brandenburg, 2006)
;
_computing_publication_material
;
SHELXL97 (Sheldrick, 2008)
;
_computing_structure_refinement
;
SHELXL97 (Sheldrick, 2008)
;
_computing_structure_solution
;
SHELXS97 (Sheldrick, 2008)
;
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 0
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Oxford Diffraction Xcalibur3 CCD'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0342
_diffrn_reflns_av_sigmaI/netI    0.0106
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       4
_diffrn_reflns_limit_l_min       -4
_diffrn_reflns_number            10399
_diffrn_reflns_theta_full        28.27
_diffrn_reflns_theta_max         28.27
_diffrn_reflns_theta_min         4.18
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    35.416
_exptl_absorpt_correction_T_max  0.632
_exptl_absorpt_correction_T_min  0.211
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
(CrysAlis RED; Oxford Diffraction, 2008)
;
_exptl_crystal_colour            grey
_exptl_crystal_density_diffrn    7.763
_exptl_crystal_density_meas      7.74
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             1484
_exptl_crystal_size_max          0.06
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.01
_refine_diff_density_max         1.764
_refine_diff_density_min         -0.985
_refine_ls_extinction_coef       0.00177(8)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method
;
SHELXL97 (Sheldrick, 2008)
;
_refine_ls_goodness_of_fit_ref   1.154
_refine_ls_matrix_type           full
_refine_ls_number_parameters     64
_refine_ls_number_reflns         670
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.154
_refine_ls_R_factor_all          0.0184
_refine_ls_R_factor_gt           0.0163
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0168P)²+3.5300P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0367
_refine_ls_wR_factor_ref         0.0376
_reflns_number_gt                623
_reflns_number_total             670
_reflns_threshold_expression     I>2sigma(I)
_cod_data_source_file            fn3196sup1.cf
_cod_data_source_block           I
_cod_database_code               2019970
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_symmetry_multiplicity
Er Er1 0.396949(18) 0.100789(18) 0.2500 0.00555(9) Uani d S 1 2
Co Co2 0.65185(6) 0.22502(6) 0.2500 0.00493(15) Uani d S 1 2
Co Co3 0.45957(6) 0.92548(6) 0.2500 0.00480(16) Uani d S 1 2
Co Co4 0.27174(5) 0.22128(6) 0.2500 0.00498(15) Uani d S 1 2
Co Co5 0.14892(5) 0.41630(6) 0.2500 0.00490(15) Uani d S 1 2
Co Co6 0.16064(18) 0.0315(2) 0.2500 0.0059(5) Uani d SP 0.51 2
Co Co7 0.12521(19) 0.0253(3) 0.2500 0.0067(5) Uani d SP 0.49 2
Si Si8 0.0000 0.0000 0.2500 0.0074(9) Uani d SP 0.50 6
Si Si9 0.44280(11) 0.76103(11) 0.2500 0.0027(3) Uani d S 1 2
Si Si10 0.13621(11) 0.25488(11) 0.2500 0.0039(3) Uani d S 1 2
Si Si11 0.43194(11) 0.37082(11) 0.2500 0.0046(3) Uani d S 1 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Er Er -0.2586 4.9576 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
Si9 Er1 Si9 7_666 7_665 78.90(4)
Si9 Er1 Si11 7_666 8 135.54(4)
Si9 Er1 Si11 7_665 8 84.64(3)
Si9 Er1 Si11 7_666 8_556 84.64(3)
Si9 Er1 Si11 7_665 8_556 135.54(4)
Si11 Er1 Si11 8 8_556 78.86(4)
Si9 Er1 Si10 7_666 8 135.54(4)
Si9 Er1 Si10 7_665 8 84.87(3)
Si11 Er1 Si10 8 8 82.67(3)
Si11 Er1 Si10 8_556 8 132.46(4)
Si9 Er1 Si10 7_666 8_556 84.87(3)
Si9 Er1 Si10 7_665 8_556 135.54(4)
Si11 Er1 Si10 8 8_556 132.46(4)
Si11 Er1 Si10 8_556 8_556 82.67(3)
Si10 Er1 Si10 8 8_556 78.39(4)
Si9 Er1 Co5 7_666 8_556 46.78(3)
Si9 Er1 Co5 7_665 8_556 95.71(3)
Si11 Er1 Co5 8 8_556 177.62(3)
Si11 Er1 Co5 8_556 8_556 102.424(19)
Si10 Er1 Co5 8 8_556 95.01(3)
Si10 Er1 Co5 8_556 8_556 46.16(3)
Si9 Er1 Co5 7_666 8 95.71(3)
Si9 Er1 Co5 7_665 8 46.78(3)
Si11 Er1 Co5 8 8 102.424(19)
Si11 Er1 Co5 8_556 8 177.62(3)
Si10 Er1 Co5 8 8 46.16(3)
Si10 Er1 Co5 8_556 8 95.01(3)
Co5 Er1 Co5 8_556 8 76.224(17)
Si9 Er1 Co3 7_666 7_666 46.63(3)
Si9 Er1 Co3 7_665 7_666 95.52(3)
Si11 Er1 Co3 8 7_666 95.20(3)
Si11 Er1 Co3 8_556 7_666 46.21(3)
Si10 Er1 Co3 8 7_666 177.79(3)
Si10 Er1 Co3 8_556 7_666 102.740(19)
Co5 Er1 Co3 8_556 7_666 87.117(16)
Co5 Er1 Co3 8 7_666 135.25(2)
Si9 Er1 Co3 7_666 7_665 95.52(3)
Si9 Er1 Co3 7_665 7_665 46.63(3)
Si11 Er1 Co3 8 7_665 46.21(3)
Si11 Er1 Co3 8_556 7_665 95.20(3)
Si10 Er1 Co3 8 7_665 102.740(19)
Si10 Er1 Co3 8_556 7_665 177.79(3)
Co5 Er1 Co3 8_556 7_665 135.25(2)
Co5 Er1 Co3 8 7_665 87.117(16)
Co3 Er1 Co3 7_666 7_665 76.065(18)
Si9 Er1 Co4 7_666 8 177.46(2)
Si9 Er1 Co4 7_665 8 103.642(19)
Si11 Er1 Co4 8 8 45.41(3)
Si11 Er1 Co4 8_556 8 93.49(3)
Si10 Er1 Co4 8 8 45.29(3)
Si10 Er1 Co4 8_556 8 93.19(3)
Co5 Er1 Co4 8_556 8 132.30(2)
Co5 Er1 Co4 8 8 86.084(16)
Co3 Er1 Co4 7_666 8 132.56(2)
Co3 Er1 Co4 7_665 8 86.352(16)
Si9 Er1 Co4 7_666 8_556 103.642(19)
Si9 Er1 Co4 7_665 8_556 177.46(2)
Si11 Er1 Co4 8 8_556 93.49(3)
Si11 Er1 Co4 8_556 8_556 45.41(3)
Si10 Er1 Co4 8 8_556 93.19(3)
Si10 Er1 Co4 8_556 8_556 45.29(3)
Co5 Er1 Co4 8_556 8_556 86.084(16)
Co5 Er1 Co4 8 8_556 132.30(2)
Co3 Er1 Co4 7_666 8_556 86.352(16)
Co3 Er1 Co4 7_665 8_556 132.56(2)
Co4 Er1 Co4 8 8_556 73.817(17)
Si11 Co2 Si9 2_655 8_556 108.30(4)
Si11 Co2 Si9 2_655 8 108.30(4)
Si9 Co2 Si9 8_556 8 100.95(6)
Si11 Co2 Si9 2_655 7_665 108.25(4)
Si9 Co2 Si9 8_556 7_665 143.45(5)
Si9 Co2 Si9 8 7_665 67.32(6)
Si11 Co2 Si9 2_655 7_666 108.25(4)
Si9 Co2 Si9 8_556 7_666 67.32(6)
Si9 Co2 Si9 8 7_666 143.45(5)
Si9 Co2 Si9 7_665 7_666 100.84(6)
Si11 Co2 Co2 2_655 2_655 150.09(6)
Si9 Co2 Co2 8_556 2_655 56.76(3)
Si9 Co2 Co2 8 2_655 56.76(3)
Si9 Co2 Co2 7_665 2_655 90.30(4)
Si9 Co2 Co2 7_666 2_655 90.30(4)
Si11 Co2 Co2 2_655 3_665 149.91(6)
Si9 Co2 Co2 8_556 3_665 90.34(4)
Si9 Co2 Co2 8 3_665 90.34(4)
Si9 Co2 Co2 7_665 3_665 56.69(4)
Si9 Co2 Co2 7_666 3_665 56.69(4)
Co2 Co2 Co2 2_655 3_665 60.0
Si11 Co2 Co3 2_655 7_665 54.56(3)
Si9 Co2 Co3 8_556 7_665 162.79(5)
Si9 Co2 Co3 8 7_665 85.05(3)
Si9 Co2 Co3 7_665 7_665 53.72(4)
Si9 Co2 Co3 7_666 7_665 116.68(4)
Co2 Co2 Co3 2_655 7_665 136.890(14)
Co2 Co2 Co3 3_665 7_665 105.86(3)
Si11 Co2 Co3 2_655 7_666 54.56(3)
Si9 Co2 Co3 8_556 7_666 85.05(3)
Si9 Co2 Co3 8 7_666 162.79(5)
Si9 Co2 Co3 7_665 7_666 116.68(4)
Si9 Co2 Co3 7_666 7_666 53.72(4)
Co2 Co2 Co3 2_655 7_666 136.890(14)
Co2 Co2 Co3 3_665 7_666 105.86(3)
Co3 Co2 Co3 7_665 7_666 84.93(3)
Si11 Co2 Co5 2_655 9_656 54.55(3)
Si9 Co2 Co5 8_556 9_656 53.76(4)
Si9 Co2 Co5 8 9_656 116.60(4)
Si9 Co2 Co5 7_665 9_656 162.75(5)
Si9 Co2 Co5 7_666 9_656 85.23(3)
Co2 Co2 Co5 2_655 9_656 105.91(3)
Co2 Co2 Co5 3_665 9_656 137.021(14)
Co3 Co2 Co5 7_665 9_656 109.11(3)
Co3 Co2 Co5 7_666 9_656 54.41(2)
Si11 Co2 Co5 2_655 9_655 54.55(3)
Si9 Co2 Co5 8_556 9_655 116.60(4)
Si9 Co2 Co5 8 9_655 53.76(4)
Si9 Co2 Co5 7_665 9_655 85.23(3)
Si9 Co2 Co5 7_666 9_655 162.75(5)
Co2 Co2 Co5 2_655 9_655 105.91(3)
Co2 Co2 Co5 3_665 9_655 137.021(14)
Co3 Co2 Co5 7_665 9_655 54.41(2)
Co3 Co2 Co5 7_666 9_655 109.11(3)
Co5 Co2 Co5 9_656 9_655 84.67(3)
Si11 Co2 Er1 2_655 2_655 83.55(4)
Si9 Co2 Er1 8_556 2_655 59.01(3)
Si9 Co2 Er1 8 2_655 59.01(3)
Si9 Co2 Er1 7_665 2_655 125.91(3)
Si9 Co2 Er1 7_666 2_655 125.91(3)
Co2 Co2 Er1 2_655 2_655 66.53(3)
Co2 Co2 Er1 3_665 2_655 126.53(3)
Co3 Co2 Er1 7_665 2_655 112.83(2)
Co3 Co2 Er1 7_666 2_655 112.83(2)
Co5 Co2 Er1 9_656 2_655 58.630(19)
Co5 Co2 Er1 9_655 2_655 58.630(19)
Si11 Co3 Si9 2_665 . 114.41(6)
Si11 Co3 Si11 2_665 8_565 110.05(4)
Si9 Co3 Si11 . 8_565 108.76(4)
Si11 Co3 Si11 2_665 8_566 110.05(4)
Si9 Co3 Si11 . 8_566 108.76(4)
Si11 Co3 Si11 8_565 8_566 104.32(6)
Si11 Co3 Co5 2_665 3_565 153.48(5)
Si9 Co3 Co5 . 3_565 92.11(5)
Si11 Co3 Co5 8_565 3_565 57.73(3)
Si11 Co3 Co5 8_566 3_565 57.73(3)
Si11 Co3 Co3 2_665 7_676 55.37(3)
Si9 Co3 Co3 . 7_676 129.84(3)
Si11 Co3 Co3 8_565 7_676 120.96(5)
Si11 Co3 Co3 8_566 7_676 54.68(4)
Co5 Co3 Co3 3_565 7_676 108.03(4)
Si11 Co3 Co3 2_665 7_675 55.37(3)
Si9 Co3 Co3 . 7_675 129.84(3)
Si11 Co3 Co3 8_565 7_675 54.68(4)
Si11 Co3 Co3 8_566 7_675 120.96(5)
Co5 Co3 Co3 3_565 7_675 108.03(4)
Co3 Co3 Co3 7_676 7_675 87.54(4)
Si11 Co3 Co2 2_665 7_665 131.79(2)
Si9 Co3 Co2 . 7_665 55.70(3)
Si11 Co3 Co2 8_565 7_665 53.08(4)
Si11 Co3 Co2 8_566 7_665 117.76(5)
Co5 Co3 Co2 3_565 7_665 62.93(2)
Co3 Co3 Co2 7_676 7_665 170.65(5)
Co3 Co3 Co2 7_675 7_665 93.019(16)
Si11 Co3 Co2 2_665 7_666 131.79(2)
Si9 Co3 Co2 . 7_666 55.70(3)
Si11 Co3 Co2 8_565 7_666 117.76(5)
Si11 Co3 Co2 8_566 7_666 53.08(4)
Co5 Co3 Co2 3_565 7_666 62.93(2)
Co3 Co3 Co2 7_676 7_666 93.019(16)
Co3 Co3 Co2 7_675 7_666 170.65(5)
Co2 Co3 Co2 7_665 7_666 84.93(3)
Si11 Co3 Er1 2_665 7_666 64.86(3)
Si9 Co3 Er1 . 7_666 64.64(3)
Si11 Co3 Er1 8_565 7_666 165.84(4)
Si11 Co3 Er1 8_566 7_666 89.80(3)
Co5 Co3 Er1 3_565 7_666 132.56(2)
Co3 Co3 Er1 7_676 7_666 68.15(2)
Co3 Co3 Er1 7_675 7_666 118.70(4)
Co2 Co3 Er1 7_665 7_666 119.29(3)
Co2 Co3 Er1 7_666 7_666 69.960(17)
Si11 Co3 Er1 2_665 7_665 64.86(3)
Si9 Co3 Er1 . 7_665 64.64(3)
Si11 Co3 Er1 8_565 7_665 89.80(3)
Si11 Co3 Er1 8_566 7_665 165.84(4)
Co5 Co3 Er1 3_565 7_665 132.56(2)
Co3 Co3 Er1 7_676 7_665 118.70(4)
Co3 Co3 Er1 7_675 7_665 68.15(2)
Co2 Co3 Er1 7_665 7_665 69.960(17)
Co2 Co3 Er1 7_666 7_665 119.29(3)
Er1 Co3 Er1 7_666 7_665 76.065(18)
Si11 Co3 Er1 2_665 1_565 85.62(4)
Si9 Co3 Er1 . 1_565 159.98(4)
Si11 Co3 Er1 8_565 1_565 61.25(3)
Si11 Co3 Er1 8_566 1_565 61.25(3)
Co5 Co3 Er1 3_565 1_565 67.87(2)
Co3 Co3 Er1 7_676 1_565 60.81(3)
Co3 Co3 Er1 7_675 1_565 60.81(3)
Co2 Co3 Er1 7_665 1_565 111.50(2)
Co2 Co3 Er1 7_666 1_565 111.50(2)
Er1 Co3 Er1 7_666 1_565 128.963(17)
Er1 Co3 Er1 7_665 1_565 128.963(17)
Si10 Co4 Si11 . . 112.59(6)
Si10 Co4 Si10 . 8 108.86(5)
Si11 Co4 Si10 . 8 110.70(4)
Si10 Co4 Si10 . 8_556 108.86(5)
Si11 Co4 Si10 . 8_556 110.70(4)
Si10 Co4 Si10 8 8_556 104.81(6)
Si10 Co4 Co6 . . 95.18(7)
Si11 Co4 Co6 . . 152.23(7)
Si10 Co4 Co6 8 . 57.01(4)
Si10 Co4 Co6 8_556 . 57.01(4)
Si10 Co4 Co6 . 9 55.01(6)
Si11 Co4 Co6 . 9 127.10(5)
Si10 Co4 Co6 8 9 53.91(7)
Si10 Co4 Co6 8_556 9 122.05(6)
Co6 Co4 Co6 . 9 68.82(8)
Si10 Co4 Co6 . 9_556 55.01(6)
Si11 Co4 Co6 . 9_556 127.10(5)
Si10 Co4 Co6 8 9_556 122.05(6)
Si10 Co4 Co6 8_556 9_556 53.91(7)
Co6 Co4 Co6 . 9_556 68.82(8)
Co6 Co4 Co6 9 9_556 89.91(9)
Si10 Co4 Co7 . . 84.86(7)
Si11 Co4 Co7 . . 162.54(7)
Si10 Co4 Co7 8 . 60.90(4)
Si10 Co4 Co7 8_556 . 60.90(4)
Co6 Co4 Co7 . . 10.31(7)
Co6 Co4 Co7 9 . 62.33(8)
Co6 Co4 Co7 9_556 . 62.33(8)
Si10 Co4 Co5 . 8_556 128.94(3)
Si11 Co4 Co5 . 8_556 55.73(3)
Si10 Co4 Co5 8 8_556 121.88(5)
Si10 Co4 Co5 8_556 8_556 54.97(4)
Co6 Co4 Co5 . 8_556 106.87(5)
Co6 Co4 Co5 9 8_556 175.02(7)
Co6 Co4 Co5 9_556 8_556 90.77(5)
Co7 Co4 Co5 . 8_556 113.78(4)
Si10 Co4 Co5 . 8 128.94(3)
Si11 Co4 Co5 . 8 55.73(3)
Si10 Co4 Co5 8 8 54.97(4)
Si10 Co4 Co5 8_556 8 121.88(5)
Co6 Co4 Co5 . 8 106.87(5)
Co6 Co4 Co5 9 8 90.77(5)
Co6 Co4 Co5 9_556 8 175.02(7)
Co7 Co4 Co5 . 8 113.78(4)
Co5 Co4 Co5 8_556 8 88.13(3)
Si10 Co4 Co7 . 9 56.86(7)
Si11 Co4 Co7 . 9 135.23(4)
Si10 Co4 Co7 8 9 52.45(7)
Si10 Co4 Co7 8_556 9 113.75(6)
Co6 Co4 Co7 . 9 60.66(8)
Co6 Co4 Co7 9 9 8.39(6)
Co6 Co4 Co7 9_556 9 85.03(5)
Co7 Co4 Co7 . 9 53.97(7)
Co5 Co4 Co7 8_556 9 167.53(6)
Co5 Co4 Co7 8 9 95.05(4)
Si10 Co4 Co7 . 9_556 56.86(7)
Si11 Co4 Co7 . 9_556 135.23(4)
Si10 Co4 Co7 8 9_556 113.75(6)
Si10 Co4 Co7 8_556 9_556 52.45(7)
Co6 Co4 Co7 . 9_556 60.66(8)
Co6 Co4 Co7 9 9_556 85.03(5)
Co6 Co4 Co7 9_556 9_556 8.39(6)
Co7 Co4 Co7 . 9_556 53.97(7)
Co5 Co4 Co7 8_556 9_556 95.05(4)
Co5 Co4 Co7 8 9_556 167.53(6)
Co7 Co4 Co7 9 9_556 79.39(7)
Si10 Co5 Si11 . 9 110.12(4)
Si10 Co5 Si11 . 9_556 110.12(4)
Si11 Co5 Si11 9 9_556 104.08(6)
Si10 Co5 Si9 . 3_565 115.05(6)
Si11 Co5 Si9 9 3_565 108.44(4)
Si11 Co5 Si9 9_556 3_565 108.44(4)
Si10 Co5 Co3 . 2_665 153.37(5)
Si11 Co5 Co3 9 2_665 57.58(3)
Si11 Co5 Co3 9_556 2_665 57.58(3)
Si9 Co5 Co3 3_565 2_665 91.59(5)
Si10 Co5 Co4 . 9 55.38(3)
Si11 Co5 Co4 9 9 54.74(4)
Si11 Co5 Co4 9_556 9 121.29(4)
Si9 Co5 Co4 3_565 9 129.72(3)
Co3 Co5 Co4 2_665 9 108.10(3)
Si10 Co5 Co4 . 9_556 55.38(3)
Si11 Co5 Co4 9 9_556 121.29(4)
Si11 Co5 Co4 9_556 9_556 54.74(4)
Si9 Co5 Co4 3_565 9_556 129.72(3)
Co3 Co5 Co4 2_665 9_556 108.10(3)
Co4 Co5 Co4 9 9_556 88.13(3)
Si10 Co5 Co2 . 8_566 132.08(2)
Si11 Co5 Co2 9 8_566 117.35(4)
Si11 Co5 Co2 9_556 8_566 52.95(4)
Si9 Co5 Co2 3_565 8_566 55.51(3)
Co3 Co5 Co2 2_665 8_566 62.66(2)
Co4 Co5 Co2 9 8_566 170.52(4)
Co4 Co5 Co2 9_556 8_566 92.843(16)
Si10 Co5 Co2 . 8_565 132.08(2)
Si11 Co5 Co2 9 8_565 52.95(4)
Si11 Co5 Co2 9_556 8_565 117.35(4)
Si9 Co5 Co2 3_565 8_565 55.51(3)
Co3 Co5 Co2 2_665 8_565 62.66(2)
Co4 Co5 Co2 9 8_565 92.843(16)
Co4 Co5 Co2 9_556 8_565 170.52(4)
Co2 Co5 Co2 8_566 8_565 84.67(3)
Si10 Co5 Er1 . 9_556 65.33(3)
Si11 Co5 Er1 9 9_556 166.01(3)
Si11 Co5 Er1 9_556 9_556 89.83(3)
Si9 Co5 Er1 3_565 9_556 64.69(3)
Co3 Co5 Er1 2_665 9_556 132.23(2)
Co4 Co5 Er1 9 9_556 119.05(3)
Co4 Co5 Er1 9_556 9_556 68.103(18)
Co2 Co5 Er1 8_566 9_556 69.881(17)
Co2 Co5 Er1 8_565 9_556 119.17(3)
Si10 Co5 Er1 . 9 65.33(3)
Si11 Co5 Er1 9 9 89.83(3)
Si11 Co5 Er1 9_556 9 166.01(3)
Si9 Co5 Er1 3_565 9 64.69(3)
Co3 Co5 Er1 2_665 9 132.23(2)
Co4 Co5 Er1 9 9 68.103(18)
Co4 Co5 Er1 9_556 9 119.05(3)
Co2 Co5 Er1 8_566 9 119.17(3)
Co2 Co5 Er1 8_565 9 69.881(17)
Er1 Co5 Er1 9_556 9 76.224(17)
Si10 Co5 Er1 . 2 87.19(4)
Si11 Co5 Er1 9 2 60.50(3)
Si11 Co5 Er1 9_556 2 60.50(3)
Si9 Co5 Er1 3_565 2 157.76(4)
Co3 Co5 Er1 2_665 2 66.18(2)
Co4 Co5 Er1 9 2 62.14(2)
Co4 Co5 Er1 9_556 2 62.14(2)
Co2 Co5 Er1 8_566 2 110.14(2)
Co2 Co5 Er1 8_565 2 110.14(2)
Er1 Co5 Er1 9_556 2 130.220(18)
Er1 Co5 Er1 9 2 130.220(18)
Si8 Co6 Si10 . 3 95.42(11)
Si8 Co6 Si10 . 8_556 114.53(8)
Si10 Co6 Si10 3 8_556 112.38(8)
Si8 Co6 Si10 . 8 114.53(8)
Si10 Co6 Si10 3 8 112.38(8)
Si10 Co6 Si10 8_556 8 107.42(13)
Si8 Co6 Co4 . . 106.31(12)
Si10 Co6 Co4 3 . 158.28(12)
Si10 Co6 Co4 8_556 . 58.57(7)
Si10 Co6 Co4 8 . 58.57(7)
Si8 Co6 Co4 . 8 119.67(8)
Si10 Co6 Co4 3 8 56.62(6)
Si10 Co6 Co4 8_556 8 125.26(10)
Si10 Co6 Co4 8 8 55.82(5)
Co4 Co6 Co4 . 8 110.26(7)
Si8 Co6 Co4 . 8_556 119.67(8)
Si10 Co6 Co4 3 8_556 56.62(6)
Si10 Co6 Co4 8_556 8_556 55.82(5)
Si10 Co6 Co4 8 8_556 125.26(10)
Co4 Co6 Co4 . 8_556 110.26(7)
Co4 Co6 Co4 8 8_556 89.91(9)
Si8 Co6 Co7 . 8 60.54(8)
Si10 Co6 Co7 3 8 60.33(9)
Si10 Co6 Co7 8_556 8 169.02(15)
Si10 Co6 Co7 8 8 83.42(5)
Co4 Co6 Co7 . 8 131.30(9)
Co4 Co6 Co7 8 8 59.20(5)
Co4 Co6 Co7 8_556 8 116.68(13)
Si8 Co6 Co7 . 8_556 60.54(8)
Si10 Co6 Co7 3 8_556 60.33(9)
Si10 Co6 Co7 8_556 8_556 83.42(5)
Si10 Co6 Co7 8 8_556 169.02(15)
Co4 Co6 Co7 . 8_556 131.30(9)
Co4 Co6 Co7 8 8_556 116.68(13)
Co4 Co6 Co7 8_556 8_556 59.20(5)
Co7 Co6 Co7 8 8_556 85.69(17)
Si8 Co6 Co7 . 9_556 60.30(8)
Si10 Co6 Co7 3 9_556 126.09(9)
Si10 Co6 Co7 8_556 9_556 55.29(5)
Si10 Co6 Co7 8 9_556 121.42(15)
Co4 Co6 Co7 . 9_556 67.44(9)
Co4 Co6 Co7 8 9_556 177.18(14)
Co4 Co6 Co7 8_556 9_556 92.44(5)
Co7 Co6 Co7 8 9_556 120.84(7)
Co7 Co6 Co7 8_556 9_556 65.95(7)
Si8 Co6 Co7 . 9 60.30(8)
Si10 Co6 Co7 3 9 126.09(9)
Si10 Co6 Co7 8_556 9 121.42(15)
Si10 Co6 Co7 8 9 55.29(5)
Co4 Co6 Co7 . 9 67.44(9)
Co4 Co6 Co7 8 9 92.44(5)
Co4 Co6 Co7 8_556 9 177.18(14)
Co7 Co6 Co7 8 9 65.95(7)
Co7 Co6 Co7 8_556 9 120.84(7)
Co7 Co6 Co7 9_556 9 85.16(16)
Si8 Co6 Co6 . 8 67.486(10)
Si10 Co6 Co6 3 8 51.38(8)
Si10 Co6 Co6 8_556 8 163.15(11)
Si10 Co6 Co6 8 8 85.44(7)
Co4 Co6 Co6 . 8 138.08(3)
Co4 Co6 Co6 8 8 53.12(9)
Co4 Co6 Co6 8_556 8 107.97(11)
Co7 Co6 Co6 8 8 9.51(5)
Co7 Co6 Co6 8_556 8 83.59(9)
Co7 Co6 Co6 9_556 8 127.34(8)
Co7 Co6 Co6 9 8 74.72(5)
Si8 Co7 Si10 . 3 106.95(16)
Si8 Co7 Co7 . 8 70.134(15)
Si10 Co7 Co7 3 8 62.36(10)
Si8 Co7 Si8 . 7 47.19(4)
Si10 Co7 Si8 3 7 101.43(10)
Co7 Co7 Si8 8 7 39.73(3)
Si8 Co7 Co7 . 9_556 70.134(15)
Si10 Co7 Co7 3 9_556 131.46(4)
Co7 Co7 Co7 8 9_556 140.27(3)
Si8 Co7 Co7 7 9_556 107.89(6)
Si8 Co7 Co7 . 8_556 70.134(15)
Si10 Co7 Co7 3 8_556 62.36(10)
Co7 Co7 Co7 8 8_556 94.37(8)
Si8 Co7 Co7 7 8_556 107.89(6)
Co7 Co7 Co7 9_556 8_556 72.11(6)
Si8 Co7 Si8 . 7_556 47.19(4)
Si10 Co7 Si8 3 7_556 101.43(10)
Co7 Co7 Si8 8 7_556 107.89(6)
Si8 Co7 Si8 7 7_556 94.37(8)
Co7 Co7 Si8 9_556 7_556 39.73(3)
Co7 Co7 Si8 8_556 7_556 39.73(3)
Si8 Co7 Co7 . 9 70.134(15)
Si10 Co7 Co7 3 9 131.46(4)
Co7 Co7 Co7 8 9 72.11(6)
Si8 Co7 Co7 7 9 39.73(3)
Co7 Co7 Co7 9_556 9 94.37(8)
Co7 Co7 Co7 8_556 9 140.27(3)
Si8 Co7 Co7 7_556 9 107.89(6)
Si8 Co7 Si10 . 8_556 124.84(9)
Si10 Co7 Si10 3 8_556 101.08(8)
Co7 Co7 Si10 8 8_556 161.88(14)
Si8 Co7 Si10 7 8_556 157.49(15)
Co7 Co7 Si10 9_556 8_556 55.80(11)
Co7 Co7 Si10 8_556 8_556 83.07(8)
Si8 Co7 Si10 7_556 8_556 81.53(4)
Co7 Co7 Si10 9 8_556 120.60(14)
Si8 Co7 Si10 . 8 124.84(9)
Si10 Co7 Si10 3 8 101.08(8)
Co7 Co7 Si10 8 8 83.07(8)
Si8 Co7 Si10 7 8 81.53(4)
Co7 Co7 Si10 9_556 8 120.60(14)
Co7 Co7 Si10 8_556 8 161.88(14)
Si8 Co7 Si10 7_556 8 157.49(15)
Co7 Co7 Si10 9 8 55.80(11)
Si10 Co7 Si10 8_556 8 93.79(10)
Si8 Co7 Co4 . . 116.95(16)
Si10 Co7 Co4 3 . 136.10(11)
Co7 Co7 Co4 8 . 132.74(4)
Si8 Co7 Co4 7 . 107.94(10)
Co7 Co7 Co4 9_556 . 68.24(10)
Co7 Co7 Co4 8_556 . 132.74(4)
Si8 Co7 Co4 7_556 . 107.94(10)
Co7 Co7 Co4 9 . 68.24(10)
Si10 Co7 Co4 8_556 . 53.62(6)
Si10 Co7 Co4 8 . 53.62(6)
Si8 Co7 Co6 . 9_556 77.23(12)
Si10 Co7 Co6 3 9_556 137.15(8)
Co7 Co7 Co6 8 9_556 146.63(13)
Si8 Co7 Co6 7 9_556 110.40(14)
Co7 Co7 Co6 9_556 9_556 9.80(7)
Co7 Co7 Co6 8_556 9_556 80.65(5)
Si8 Co7 Co6 7_556 9_556 49.53(6)
Co7 Co7 Co6 9 9_556 90.70(11)
Si10 Co7 Co6 8_556 9_556 50.78(5)
Si10 Co7 Co6 8 9_556 111.14(12)
Co4 Co7 Co6 . 9_556 58.47(7)
Co7 Si8 Co7 3 2 120.0
Co7 Si8 Co7 3 . 120.0
Co7 Si8 Co7 2 . 120.0
Co7 Si8 Si8 3 7_556 90.0
Co7 Si8 Si8 2 7_556 90.0
Co7 Si8 Si8 . 7_556 90.0
Co7 Si8 Si8 3 7 90.0
Co7 Si8 Si8 2 7 90.0
Co7 Si8 Si8 . 7 90.0
Si8 Si8 Si8 7_556 7 180.0
Co7 Si8 Co6 3 3 0.33(19)
Co7 Si8 Co6 2 3 119.67(19)
Co7 Si8 Co6 . 3 120.33(19)
Si8 Si8 Co6 7_556 3 90.0
Si8 Si8 Co6 7 3 90.0
Co7 Si8 Co6 3 2 120.33(19)
Co7 Si8 Co6 2 2 0.33(19)
Co7 Si8 Co6 . 2 119.67(19)
Si8 Si8 Co6 7_556 2 90.0
Si8 Si8 Co6 7 2 90.0
Co6 Si8 Co6 3 2 120.0
Co7 Si8 Co6 3 . 119.67(19)
Co7 Si8 Co6 2 . 120.33(19)
Co7 Si8 Co6 . . 0.33(19)
Si8 Si8 Co6 7_556 . 90.0
Si8 Si8 Co6 7 . 90.0
Co6 Si8 Co6 3 . 120.0
Co6 Si8 Co6 2 . 120.0
Co7 Si8 Co7 3 9_556 132.81(4)
Co7 Si8 Co7 2 9_556 70.134(15)
Co7 Si8 Co7 . 9_556 70.135(15)
Si8 Si8 Co7 7_556 9_556 42.81(4)
Si8 Si8 Co7 7 9_556 137.19(4)
Co6 Si8 Co7 3 9_556 132.81(4)
Co6 Si8 Co7 2 9_556 69.93(12)
Co6 Si8 Co7 . 9_556 70.34(12)
Co7 Si8 Co7 3 7 70.134(15)
Co7 Si8 Co7 2 7 70.135(15)
Co7 Si8 Co7 . 7 132.81(4)
Si8 Si8 Co7 7_556 7 137.19(4)
Si8 Si8 Co7 7 7 42.81(4)
Co6 Si8 Co7 3 7 69.93(12)
Co6 Si8 Co7 2 7 70.34(12)
Co6 Si8 Co7 . 7 132.81(4)
Co7 Si8 Co7 9_556 7 140.27(3)
Co7 Si8 Co7 3 8 70.134(15)
Co7 Si8 Co7 2 8 132.81(4)
Co7 Si8 Co7 . 8 70.135(15)
Si8 Si8 Co7 7_556 8 137.19(4)
Si8 Si8 Co7 7 8 42.81(4)
Co6 Si8 Co7 3 8 70.34(12)
Co6 Si8 Co7 2 8 132.81(4)
Co6 Si8 Co7 . 8 69.93(12)
Co7 Si8 Co7 9_556 8 140.27(3)
Co7 Si8 Co7 7 8 72.11(6)
Co7 Si8 Co7 3 8_556 70.135(15)
Co7 Si8 Co7 2 8_556 132.81(4)
Co7 Si8 Co7 . 8_556 70.135(15)
Si8 Si8 Co7 7_556 8_556 42.81(4)
Si8 Si8 Co7 7 8_556 137.19(4)
Co6 Si8 Co7 3 8_556 70.34(12)
Co6 Si8 Co7 2 8_556 132.81(4)
Co6 Si8 Co7 . 8_556 69.93(12)
Co7 Si8 Co7 9_556 8_556 72.11(6)
Co7 Si8 Co7 7 8_556 140.27(3)
Co7 Si8 Co7 8 8_556 94.37(8)
Co3 Si9 Co5 . 2_665 123.70(6)
Co3 Si9 Co2 . 9 129.48(3)
Co5 Si9 Co2 2_665 9 70.73(4)
Co3 Si9 Co2 . 9_556 129.48(3)
Co5 Si9 Co2 2_665 9_556 70.73(4)
Co2 Si9 Co2 9 9_556 100.95(6)
Co3 Si9 Co2 . 7_665 70.58(4)
Co5 Si9 Co2 2_665 7_665 129.54(3)
Co2 Si9 Co2 9 7_665 66.55(3)
Co2 Si9 Co2 9_556 7_665 142.29(7)
Co3 Si9 Co2 . 7_666 70.58(4)
Co5 Si9 Co2 2_665 7_666 129.54(3)
Co2 Si9 Co2 9 7_666 142.29(7)
Co2 Si9 Co2 9_556 7_666 66.55(3)
Co2 Si9 Co2 7_665 7_666 100.84(6)
Co3 Si9 Si9 . 3_565 148.01(8)
Co5 Si9 Si9 2_665 3_565 88.30(8)
Co2 Si9 Si9 9 3_565 56.37(4)
Co2 Si9 Si9 9_556 3_565 56.37(4)
Co2 Si9 Si9 7_665 3_565 89.66(4)
Co2 Si9 Si9 7_666 3_565 89.66(4)
Co3 Si9 Si9 . 2_665 88.01(8)
Co5 Si9 Si9 2_665 2_665 148.30(8)
Co2 Si9 Si9 9 2_665 89.70(4)
Co2 Si9 Si9 9_556 2_665 89.70(4)
Co2 Si9 Si9 7_665 2_665 56.31(4)
Co2 Si9 Si9 7_666 2_665 56.31(4)
Si9 Si9 Si9 3_565 2_665 60.0
Co3 Si9 Er1 . 7_666 68.73(3)
Co5 Si9 Er1 2_665 7_666 68.53(3)
Co2 Si9 Er1 9 7_666 137.68(6)
Co2 Si9 Er1 9_556 7_666 76.06(2)
Co2 Si9 Er1 7_665 7_666 137.70(6)
Co2 Si9 Er1 7_666 7_666 76.12(2)
Si9 Si9 Er1 3_565 7_666 131.97(5)
Si9 Si9 Er1 2_665 7_666 131.96(5)
Co3 Si9 Er1 . 7_665 68.73(3)
Co5 Si9 Er1 2_665 7_665 68.53(3)
Co2 Si9 Er1 9 7_665 76.06(2)
Co2 Si9 Er1 9_556 7_665 137.68(6)
Co2 Si9 Er1 7_665 7_665 76.12(2)
Co2 Si9 Er1 7_666 7_665 137.70(6)
Si9 Si9 Er1 3_565 7_665 131.97(5)
Si9 Si9 Er1 2_665 7_665 131.96(5)
Er1 Si9 Er1 7_666 7_665 78.90(4)
Co6 Si10 Co6 2 9 78.34(10)
Co6 Si10 Co6 2 9_556 78.34(10)
Co6 Si10 Co6 9 9_556 107.42(13)
Co6 Si10 Co4 2 . 123.10(9)
Co6 Si10 Co4 9 . 69.16(8)
Co6 Si10 Co4 9_556 . 69.16(8)
Co6 Si10 Co5 2 . 110.15(9)
Co6 Si10 Co5 9 . 126.29(6)
Co6 Si10 Co5 9_556 . 126.29(6)
Co4 Si10 Co5 . . 126.75(7)
Co6 Si10 Co4 2 9 69.47(5)
Co6 Si10 Co4 9 9 64.41(7)
Co6 Si10 Co4 9_556 9 147.72(9)
Co4 Si10 Co4 . 9 127.57(3)
Co5 Si10 Co4 . 9 69.65(4)
Co6 Si10 Co4 2 9_556 69.47(5)
Co6 Si10 Co4 9 9_556 147.72(9)
Co6 Si10 Co4 9_556 9_556 64.41(7)
Co4 Si10 Co4 . 9_556 127.57(3)
Co5 Si10 Co4 . 9_556 69.65(4)
Co4 Si10 Co4 9 9_556 104.81(6)
Co6 Si10 Co7 2 2 11.86(6)
Co6 Si10 Co7 9 2 71.82(9)
Co6 Si10 Co7 9_556 2 71.82(9)
Co4 Si10 Co7 . 2 111.24(9)
Co5 Si10 Co7 . 2 122.01(9)
Co4 Si10 Co7 9 2 76.07(5)
Co4 Si10 Co7 9_556 2 76.07(5)
Co6 Si10 Co7 2 9 68.89(9)
Co6 Si10 Co7 9 9 10.16(6)
Co6 Si10 Co7 9_556 9 101.11(8)
Co4 Si10 Co7 . 9 73.16(8)
Co5 Si10 Co7 . 9 132.01(6)
Co4 Si10 Co7 9 9 65.48(7)
Co4 Si10 Co7 9_556 9 137.90(9)
Co7 Si10 Co7 2 9 61.84(8)
Co6 Si10 Co7 2 9_556 68.89(9)
Co6 Si10 Co7 9 9_556 101.11(8)
Co6 Si10 Co7 9_556 9_556 10.16(6)
Co4 Si10 Co7 . 9_556 73.16(8)
Co5 Si10 Co7 . 9_556 132.01(6)
Co4 Si10 Co7 9 9_556 137.90(9)
Co4 Si10 Co7 9_556 9_556 65.48(7)
Co7 Si10 Co7 2 9_556 61.84(8)
Co7 Si10 Co7 9 9_556 93.79(10)
Co6 Si10 Er1 2 9_556 140.11(2)
Co6 Si10 Er1 9 9_556 136.46(9)
Co6 Si10 Er1 9_556 9_556 72.91(6)
Co4 Si10 Er1 . 9_556 70.85(4)
Co5 Si10 Er1 . 9_556 68.51(3)
Co4 Si10 Er1 9 9_556 135.70(6)
Co4 Si10 Er1 9_556 9_556 73.39(3)
Co7 Si10 Er1 2 9_556 140.650(19)
Co7 Si10 Er1 9 9_556 143.22(9)
Co7 Si10 Er1 9_556 9_556 83.00(5)
Co6 Si10 Er1 2 9 140.11(2)
Co6 Si10 Er1 9 9 72.91(6)
Co6 Si10 Er1 9_556 9 136.46(9)
Co4 Si10 Er1 . 9 70.85(4)
Co5 Si10 Er1 . 9 68.51(3)
Co4 Si10 Er1 9 9 73.39(3)
Co4 Si10 Er1 9_556 9 135.70(6)
Co7 Si10 Er1 2 9 140.650(19)
Co7 Si10 Er1 9 9 83.00(5)
Co7 Si10 Er1 9_556 9 143.22(9)
Er1 Si10 Er1 9_556 9 78.39(4)
Co2 Si11 Co4 3_665 . 116.07(6)
Co2 Si11 Co3 3_665 3_565 116.42(6)
Co4 Si11 Co3 . 3_565 127.50(7)
Co2 Si11 Co3 3_665 9_656 72.36(4)
Co4 Si11 Co3 . 9_656 127.75(3)
Co3 Si11 Co3 3_565 9_656 69.95(4)
Co2 Si11 Co3 3_665 9_655 72.36(4)
Co4 Si11 Co3 . 9_655 127.75(3)
Co3 Si11 Co3 3_565 9_655 69.95(4)
Co3 Si11 Co3 9_656 9_655 104.32(6)
Co2 Si11 Co5 3_665 8 72.50(4)
Co4 Si11 Co5 . 8 69.53(4)
Co3 Si11 Co5 3_565 8 127.91(3)
Co3 Si11 Co5 9_656 8 144.86(7)
Co3 Si11 Co5 9_655 8 64.68(3)
Co2 Si11 Co5 3_665 8_556 72.50(4)
Co4 Si11 Co5 . 8_556 69.53(4)
Co3 Si11 Co5 3_565 8_556 127.91(3)
Co3 Si11 Co5 9_656 8_556 64.68(3)
Co3 Si11 Co5 9_655 8_556 144.86(7)
Co5 Si11 Co5 8 8_556 104.08(6)
Co2 Si11 Er1 3_665 9 140.553(18)
Co4 Si11 Er1 . 9 71.12(4)
Co3 Si11 Er1 3_565 9 68.93(3)
Co3 Si11 Er1 9_656 9 136.57(6)
Co3 Si11 Er1 9_655 9 73.92(2)
Co5 Si11 Er1 8 9 74.99(2)
Co5 Si11 Er1 8_556 9 137.94(6)
Co2 Si11 Er1 3_665 9_556 140.553(18)
Co4 Si11 Er1 . 9_556 71.12(4)
Co3 Si11 Er1 3_565 9_556 68.93(3)
Co3 Si11 Er1 9_656 9_556 73.92(2)
Co3 Si11 Er1 9_655 9_556 136.57(6)
Co5 Si11 Er1 8 9_556 137.94(6)
Co5 Si11 Er1 8_556 9_556 74.99(2)
Er1 Si11 Er1 9 9_556 78.86(4)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Er1 Si9 7_666 2.8997(11)
Er1 Si9 7_665 2.8997(11)
Er1 Si11 8 2.9010(11)
Er1 Si11 8_556 2.9010(11)
Er1 Si10 8 2.9155(11)
Er1 Si10 8_556 2.9155(11)
Er1 Co5 8_556 2.9853(6)
Er1 Co5 8 2.9853(6)
Er1 Co3 7_666 2.9905(6)
Er1 Co3 7_665 2.9905(6)
Er1 Co4 8 3.0681(6)
Er1 Co4 8_556 3.0681(6)
Co2 Si11 2_655 2.2896(15)
Co2 Si9 8_556 2.3887(10)
Co2 Si9 8 2.3887(10)
Co2 Si9 7_665 2.3906(10)
Co2 Si9 7_666 2.3906(10)
Co2 Co2 2_655 2.6223(13)
Co2 Co2 3_665 2.6223(13)
Co2 Co3 7_665 2.7291(7)
Co2 Co3 7_666 2.7291(7)
Co2 Co5 9_656 2.7359(7)
Co2 Co5 9_655 2.7359(7)
Co2 Er1 2_655 3.2830(8)
Co3 Si11 2_665 2.3134(16)
Co3 Si9 . 2.3328(15)
Co3 Si11 8_565 2.3330(10)
Co3 Si11 8_566 2.3330(10)
Co3 Co5 3_565 2.4983(11)
Co3 Co3 7_676 2.6635(10)
Co3 Co3 7_675 2.6635(10)
Co3 Co2 7_665 2.7291(7)
Co3 Co2 7_666 2.7291(7)
Co3 Er1 7_666 2.9905(6)
Co3 Er1 7_665 2.9905(6)
Co3 Er1 1_565 3.1795(8)
Co4 Si10 . 2.3083(16)
Co4 Si11 . 2.3092(15)
Co4 Si10 8 2.3253(10)
Co4 Si10 8_556 2.3253(10)
Co4 Co6 . 2.458(3)
Co4 Co6 9 2.608(2)
Co4 Co6 9_556 2.608(2)
Co4 Co7 . 2.628(3)
Co4 Co5 8_556 2.6493(7)
Co4 Co5 8 2.6493(7)
Co4 Co7 9 2.885(2)
Co4 Co7 9_556 2.885(2)
Co5 Si10 . 2.3138(16)
Co5 Si11 9 2.3369(10)
Co5 Si11 9_556 2.3369(10)
Co5 Si9 3_565 2.3376(15)
Co5 Co3 2_665 2.4983(11)
Co5 Co4 9 2.6493(7)
Co5 Co4 9_556 2.6493(7)
Co5 Co2 8_566 2.7359(7)
Co5 Co2 8_565 2.7359(7)
Co5 Er1 9_556 2.9853(6)
Co5 Er1 9 2.9853(6)
Co5 Er1 2 3.2195(7)
Co6 Si8 . 2.194(2)
Co6 Si10 3 2.250(3)
Co6 Si10 8_556 2.2859(18)
Co6 Si10 8 2.2859(18)
Co6 Co4 8 2.608(2)
Co6 Co4 8_556 2.608(2)
Co6 Co7 8 2.709(4)
Co6 Co7 8_556 2.709(4)
Co6 Co7 9_556 2.723(4)
Co6 Co7 9 2.723(4)
Co6 Co6 8 2.8653(17)
Co7 Si8 . 1.707(2)
Co7 Si10 3 2.356(4)
Co7 Co7 8 2.5117(16)
Co7 Si8 7 2.5117(16)
Co7 Co7 9_556 2.5117(16)
Co7 Co7 8_556 2.5117(16)
Co7 Si8 7_556 2.5117(16)
Co7 Co7 9 2.5117(16)
Co7 Si10 8_556 2.524(2)
Co7 Si10 8 2.524(2)
Co7 Co6 9_556 2.709(4)
Si8 Co7 3 1.707(2)
Si8 Co7 2 1.707(2)
Si8 Si8 7_556 1.8425
Si8 Si8 7 1.8425
Si8 Co6 3 2.194(2)
Si8 Co6 2 2.194(2)
Si8 Co7 9_556 2.5117(16)
Si8 Co7 7 2.5117(16)
Si8 Co7 8 2.5117(16)
Si8 Co7 8_556 2.5117(16)
Si9 Co5 2_665 2.3376(15)
Si9 Co2 9 2.3887(10)
Si9 Co2 9_556 2.3887(10)
Si9 Co2 7_665 2.3906(10)
Si9 Co2 7_666 2.3906(10)
Si9 Si9 3_565 2.649(2)
Si9 Si9 2_665 2.649(2)
Si9 Er1 7_666 2.8997(11)
Si9 Er1 7_665 2.8997(11)
Si10 Co6 2 2.250(3)
Si10 Co6 9 2.2859(18)
Si10 Co6 9_556 2.2859(18)
Si10 Co4 9 2.3253(10)
Si10 Co4 9_556 2.3253(10)
Si10 Co7 2 2.356(4)
Si10 Co7 9 2.524(2)
Si10 Co7 9_556 2.524(2)
Si10 Er1 9_556 2.9155(11)
Si10 Er1 9 2.9155(11)
Si11 Co2 3_665 2.2896(15)
Si11 Co3 3_565 2.3134(16)
Si11 Co3 9_656 2.3330(10)
Si11 Co3 9_655 2.3330(10)
Si11 Co5 8 2.3369(10)
Si11 Co5 8_556 2.3369(10)
Si11 Er1 9 2.9010(11)
Si11 Er1 9_556 2.9010(11)

_cod_database_fobs_code 2019970
